Ba2M(C3N3O3)2 (M = Mg, Ca): potential UV birefringent materials with strengthened optical anisotropy originating from the (C3N3O3)3− group
Li, Zhuang; Liang, Fei; Guo, Yangwu; Lin, Zheshuai; Yao, Jiyong; Zhang, Guochun; Yin, Wenlong; Wu, Yicheng; Chen, Chuangtian; Journal of Materials Chemistry C 6 (2018) 12879–; doi:10.1039/C8TC04710C

data_7237522
_publ_section_title
;
 Ba2M(C3N3O3)2 (M = Mg, Ca): potential UV birefringent materials with
 strengthened optical anisotropy originating from the (C3N3O3)3&#x2212;
 group
;
_journal_issue                   47
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              12879
_journal_paper_doi               10.1039/C8TC04710C
_journal_volume                  6
_journal_year                    2018
_chemical_formula_moiety         '0.33(C18 Ba6 Mg3 N18 O18)'
_chemical_formula_sum            'C6 Ba2 Mg N6 O6'
_chemical_formula_weight         551.06
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_Int_Tables_number      148
_atom_sites_solution_primary     direct
_audit_creation_date             2018-05-16
_audit_creation_method
;
Olex2 1.2
(compiled 2017.08.10 svn.r3458 for OlexSys, GUI svn.r5381)
;
_audit_update_record
;
2018-07-16 deposited with the CCDC.
2018-10-18 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   6.9794(3)
_cell_length_b                   6.9794(3)
_cell_length_c                   16.9761(12)
_cell_measurement_reflns_used    5710
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      31.037
_cell_measurement_theta_min      3.578
_cell_volume                     716.15(7)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2015)'
_computing_structure_solution    'SIR2004 (Burla et al., 2007)'
_diffrn_ambient_temperature      153(2)
_diffrn_measured_fraction_theta_full 1.0000
_diffrn_measured_fraction_theta_max 1.0000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0768
_diffrn_reflns_av_unetI/netI     0.0267
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            5151
_diffrn_reflns_theta_full        26.3516
_diffrn_reflns_theta_max         26.35
_diffrn_reflns_theta_min         3.58
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    8.312
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.3215
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.8330
_exptl_crystal_description       prism
_exptl_crystal_F_000             749.5236
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         0.5367
_refine_diff_density_min         -0.7599
_refine_diff_density_rms         0.1663
_refine_ls_d_res_high            0.8006
_refine_ls_d_res_low             5.6942
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.2629
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     34
_refine_ls_number_reflns         326
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.2629
_refine_ls_R_factor_all          0.0196
_refine_ls_R_factor_gt           0.0173
_refine_ls_shift/su_max          0.0007
_refine_ls_shift/su_mean         0.0003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0200P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0439
_refine_ls_wR_factor_ref         0.0474
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              7
_reflns_limit_h_min              0
_reflns_limit_k_max              7
_reflns_limit_k_min              0
_reflns_limit_l_max              21
_reflns_limit_l_min              -20
_reflns_number_gt                310
_reflns_number_total             326
_reflns_threshold_expression     I>=2u(I)
_cod_data_source_file            c8tc04710c2.cif
_cod_data_source_block           xin
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               7237522
_olex2_refinement_description
;
;
_olex2_submission_special_instructions 'No special instructions were received'